Loading in 2 Seconds...
Loading in 2 Seconds...
Lecture 8 Chemical/Electronic Structure of Glass Syllabus Topic 6. Electronic spectroscopy studies of glass structure. Fundamentals and Applications of X-ray Photoelectron Spectroscopy (XPS) a.k.a. Electron Spectroscopy for Chemical Analysis (ESCA). Review of Lecture 7.
Fundamentals and Applications of
X-ray Photoelectron Spectroscopy (XPS)
a.k.a. Electron Spectroscopy for Chemical Analysis (ESCA)
XPS data come with Auger as by-product.
XPS of solids consists of core levels and valence band.
Intensity of core levels decreases with decreasing BE.
BE of a given level is unique to the particular element.
ARXPS allows depth profile by varying the angle between the detector and sample surface normal.
XPS probes <10 nm of the surface region.
The area under the peak of a core level peak is directly proportional to the concentration of that particular element.
Free atomsChemical Structure by XPSCharge potential model for bonds
Consider valence electrons as hollow charged sphere. Neglecting relaxation effects:
Ei = Ei0 + qi/rv+ i=j qi/rij
Ei = qi/rv+ (i=j qi/rij)
qi for valence electrons => change in energy of all inner level by qi/rv where rv is the valence shell radius.
Map the peaks for the four kinds of C in the molecule!
C 1s spectrum of ethyl trifluoroacetate
A deconvolution procedure may be needed when the components are not resolved.
To obtain unique decomposition of spectrum, additional information may be required, including estimates from ab initio simulations.
O 1s spectrum of sodium silicate glass
What do the two ?? marked peaks represent?
C. H. Hsieh et al. J. Non-cryst. Solids 168, 247-257 (1994).
What question was raised earlier in the course with regard to the difference in the structure of alkali silicates and germanates?
Nanba and Miura
Addition of alkali means two choices:
Creation of NBO as in silicates
Change of Ge from tetrahedral to octahedral coordination
Xu et al. Phys Chem Glass (1996)
533.0 Polycrystalline powder of stishovite, natural mineral from meteor crater Arizona, the densest modification of SiO2
532.9 pelletized, composition determined by XPS is SiO2.08
533.8 Thermal oxide - SiO2.1.
532.7 Thermaly grown SiO2
532.7 Fused quartz.
532.8 alpha phase, insulator, polycrystalline
533.2 Quartz (rock crystal).
532.0 Polycrystalline powder of stishovite from meteor crater, Arizona
NIST X-ray Photoelectron Spectroscopy Database: http://srdata.nist.gov/xps/
Charging of surface
Error in BE
Error in composition
Damage by sputtering (if used in depth analysis)
Alteration of structure
Net build up of charge on the surface when e loss is not compensated by inward flow => Surface at unknown +V =>
All peaks shifted/broadened by ~ the same amount.
Problem mostly corrected by flooding with low energy e.
For precise b.e. values, need a reference:
1. Adventitious C-1s (may not be present on pristine surface)
2. Thin overlayer of Au
3. Internal reference e.g. Si-2p in silicate glasses.
4. Use Auger parameter
Soda-Lime-Silicate Glass 13.30Na2O 11.62CaO 73.86SiO2 (mole %)
X-irradiation is the primary cause for Na accumulation. Once liberated, Na can migrate to the surface very quickly, if e-field is present.
The loss of oxygen is mostly determined by x-ray dose; electrons retard it.
• Elements detected from Li to U.
• Nondestructive (x-ray beam damage in certain materials?)
• Chemical bonding (e-density) analysis.
• Surface sensitivity from 5 to 75 angstroms.
• Conducting and insulating materials.
• Detection limits that range form 0.01 to 0.5 atom percent.
• Spatial resolution for surface mapping from >10 mm.
• Depth profiling (non-destructive as well as destructive).